- Home
- Documents
*Colloidal quasicrystals with 12-fold and 18-fold ...Colloidal quasicrystals with 12-fold and 18-fold...*

Click here to load reader

View

17Download

0

Embed Size (px)

Colloidal quasicrystals with 12-fold and18-fold diffraction symmetrySteffen Fischera, Alexander Exnera, Kathrin Zielskea, Jan Perlichb, Sofia Deloudic, Walter Steurerc,Peter Lindnerd, and Stephan Förstere,1

aInstitut für Physikalische Chemie, Universität Hamburg, D-20146 Hamburg, Germany; bHamburger Synchrotronstrahlungslabor/Deutsches ElektronenSynchrotron, D-22607 Hamburg, Germany; cLaboratory of Crystallography, Department of Materials, Eidgenössiche Technische Hochschule Zürich,CH-8093 Zürich, Switzerland; dInstitut Laue Langevin, F-38042 Grenoble Cedex 9, France; and ePhysikalische Chemie I, University of Bayreuth,D-95447 Bayreuth, Germany

Edited by Noel A. Clark, University of Colorado at Boulder, Boulder, CO, and approved December 9, 2010 (received for review June 18, 2010)

Micelles are the simplest example of self-assembly found in nature.As many other colloids, they can self-assemble in aqueous solutionto form ordered periodic structures. These structures so far allexhibited classical crystallographic symmetries. Here we reportthat micelles in solution can self-assemble into quasicrystallinephases. We observe phases with 12-fold and 18-fold diffractionsymmetry. Colloidal water-based quasicrystals are physically andchemically very simple systems. Macroscopic monodomain samplesof centimeter dimension can be easily prepared. Phase transitionsbetween the fcc phase and the two quasicrystalline phases can beeasily followed in situ by time-resolved diffraction experiments.The discovery of quasicrystalline colloidal solutions advances thetheoretical understanding of quasicrystals considerably, as forthese systems the stability of quasicrystalline states has beentheoretically predicted for the concentration and temperaturerange, where they are experimentally observed. Also for the use ofquasicrystals in advanced materials this discovery is of particularimportance, as it opens the route to quasicrystalline photonic bandgap materials via established water-based colloidal self-assemblytechniques.

Micelles are the simplest type of self-assembly structurefound in nature. They are formed by the association ofamphiphilic molecules in solution. Micelles are ubiquitous col-loids being used in washing detergents, for the solubilizationof pharmaceuticals as well as for the preparation of advancedmaterials (1). Above concentrations of about 10%, there is anorder–disorder transition, where micelles self-assemble intoliquid crystalline structures. In the case of spherical micelles, themost common structure types are of cubic symmetry with spacegroups Fm3̄m (fcc) or Im3̄m (body-centered cubic).

We were investigating the liquid crystalline phase behavior ofpolymeric micelles in this concentration range in greater detail.For this investigation we used block copolymer micelles thathave a well-defined micellar core containing the hydrophobicpolymer blocks, surrounded by a relatively large shell consistingof the hydrophilic polymer blocks. As block copolymers we usedpolyðisoprene-b-ethylene oxideÞ, PIn-PEOm, with different de-grees of polymerization n andm of the respective polymer blocks.By shear orientation using plate–plate or Searle-type rheometers,large monodomain samples of centimeter dimension can be pre-pared that allows one to determine the liquid crystalline structureby using small-angle X-ray scattering (SAXS) and small-angleneutron scattering (SANS) (2).

ResultsWhen investigating the phase behavior of PI30-PEO120 micellesnear the order–disorder transition with synchrotron SAXSand SANS, we discovered phases with diffraction patterns of12- (Q12) and 18-fold (Q18) diffraction symmetry (Fig. 1). Withincreasing concentration we find at a temperature of 20 °C asequence of phases Disordered j13%jQ12j18%j Cubic (fcc). Inthe concentration range between 13 and 18%, we observe theQ12-phase to be stable at intermediate temperatures (15° and

20 °C), the Q18 phase to be stable at lower temperatures (10 °C),and the fcc phase to be stable at temperatures equal to and above25 °C. In the scattering curves of isotropic samples in the concen-tration range between 14–20% at 20 °C the phase transition fcc →Q12 is evident only from the suppression of the 110 reflection andthe development of a weak maximum at q ¼ 0.45 nm−1 (seeFig. 2). Each of the scattering curves in Fig. 2 has been measuredat a synchrotron beamline (BW4, DESY) by successive exposuresof 30-min duration (to check for possible beam damage) using aPilatus 300-k detector. Measurements over a broader concentra-tion range between 10–25% have been performed with lowerresolution and are shown in SI Text. From the peak positionsand the positions of the form factor oscillations in the scatteringcurve of the fcc phase, we calculate a unit cell dimension of52.2 nm and a radius of the micellar core of 8.1 nm.

Fig. 1 shows the diffraction patterns of shear-oriented samplesfor the Q12, Q18, and fcc phases. For the Q12 phase we observe adiffraction pattern with 12-fold symmetry (Fig. 1B), for the Q18phase with 18-fold symmetry (Fig. 1C). The diffraction pattern ofthe fcc phase is characterized by a 6-fold diffraction symmetrywith pronounced 220 reflections (Fig. 1A). The full diffractionpattern of the Q12 phase measured with a larger area detectoris shown in SI Text. The Q12 phase was also studied by SANS,and the diffraction pattern with the characteristic 12-fold diffrac-tion symmetry is shown in Fig. 1D. In addition, the diffraction inthe orthogonal direction was determined and is shown in Fig. 1E.The Q12 and Q18 phases are stable after shearing. When scan-ning with the beam (20 × 40 μm) through the sample (30-mm dia-meter), the same diffraction patterns are found. We reproducedthe results by synthesizing further block copolymers with similarblock lengths, i.e., PI30-PEO124 and PI32-PEO120 that showedexactly the same behavior.

To get insight into the topological changes during the phasetransition from fcc into the Q12 and Q18 phase, we performedtime-resolved microfocus synchrotron SAXS experiments. Thesample, a micellar PI30-PEO120 solution at 15%, was cooled un-der oscillatory shear to induce phase transitions from a fcc mono-domain into the Q12 and the Q18 phase. Diffraction patternswere recorded in 10-s frames and are shown in Fig. 3. At thebeginning we observe the characteristic diffraction pattern of thefcc phase with its 6-fold diffraction symmetry. The strong 220reflections, but also the weak 222 reflections, are observed. In thesecond diffraction pattern, measured after 10 s, a second set of six

Author contributions: S. Forster designed research; S. Fischer, A.E., and K.Z. performedresearch; J.P. and P.L. contributed new reagents/analytic tools; S.D., W.S., and S. Forsteranalyzed data; and S. Forster wrote the paper.

The authors declare no conflict of interest.

This article is a PNAS Direct Submission.1To whom correspondence should be addressed. E-mail: [email protected]

This article contains supporting information online at www.pnas.org/lookup/suppl/doi:10.1073/pnas.1008695108/-/DCSupplemental.

1810–1814 ∣ PNAS ∣ February 1, 2011 ∣ vol. 108 ∣ no. 5 www.pnas.org/cgi/doi/10.1073/pnas.1008695108

Dow

nloa

ded

by g

uest

on

July

7, 2

020

http://www.pnas.org/lookup/suppl/doi:10.1073/pnas.1008695108/-/DCSupplemental/pnas.1008695108_SI.pdf?targetid=STXThttp://www.pnas.org/lookup/suppl/doi:10.1073/pnas.1008695108/-/DCSupplemental/pnas.1008695108_SI.pdf?targetid=STXThttp://www.pnas.org/lookup/suppl/doi:10.1073/pnas.1008695108/-/DCSupplementalhttp://www.pnas.org/lookup/suppl/doi:10.1073/pnas.1008695108/-/DCSupplementalhttp://www.pnas.org/lookup/suppl/doi:10.1073/pnas.1008695108/-/DCSupplementalhttp://www.pnas.org/lookup/suppl/doi:10.1073/pnas.1008695108/-/DCSupplementalhttp://www.pnas.org/lookup/suppl/doi:10.1073/pnas.1008695108/-/DCSupplementalhttp://www.pnas.org/lookup/suppl/doi:10.1073/pnas.1008695108/-/DCSupplemental

strong reflections (62) has appeared between the six 220 reflec-tions (61), indicated by the arrow. This signals the transition intothe Q12 phase. After 40 s the Q12 phase has fully developed.After 50 s the transition into the Q18 phase has started indicatedby the splitting of the six (61) reflections (see arrows in Fig. 3),which subsequently develop into two peaks separated by anazimuthal angle of 20°. The position of the six (62) reflectionsremains unchanged during this rearrangement. This results inthe diffraction pattern of the Q18 phase with its 18-fold diffrac-tion symmetry. During phase transitions there is a significantincrease in forward scattering due to the heterogeneities of thebiphasic regions.

The observed crystallographically “forbidden” diffractionpatterns with 12-fold and 18-fold diffraction symmetry could be

the result of the formation of a quasicrystalline phase, but couldalso be due to the presence of a twinned fcc polydomain struc-ture. The time-resolved experiments suggest that the transitionfrom the fcc phase (Fm3̄m) to the Q12 and Q18 phases proceedsvia rearrangements of micelles in the (111) layers of the fccphase. Such rearrangements could result in a 30° rotation of the(111) layers. For a multidomain structure consisting of the samenumber of 30°-rotated and -unrotated layers this would give riseto diffraction patterns with 12-fold rotational symmetry in the[111] direction. To be consistent with the mirror symmetry ofthe diffraction pattern observed in the perpendicular direction(Fig. 1E), domains of layers with ABCA… stacking as well as do-mains with the corresponding twinned ACBA… stacking shouldbe present with equal probability. To calculate the correspondingdiffraction patterns we considered a multidomain structure con-sisting of sequences ðABCÞnðA0B0C0ÞnðACBÞnðA0C0B0Þn of layersthat contain the structural features of equal numbers of twinnedand 30°-rotated/-nonrotated layers. This layer stacking is shownin Fig. 4E. The subscript n denotes the number of layer repeti-tions and the primes indicate 30°-rotated layers. We find that thediffraction patterns for n ¼ 2, parallel and perpendicular to the(111) layers, are very similar to the diffraction patterns calculatedfor other stacking sequences.

Because of the sixfold symmetry the stacking of alternate0°;30°;0°;…-rotated domains is equal to a stacking of 0°;30°;60°;…-rotated domains, which would be conceptually very similarto the structure of smectic twisted grain boundary (TGB) phases.The TGB phase consists of smectic grains separated by twistedgrain boundaries. If the angle α between the layer normals inadjacent slabs is a rational number P/Q, then the TGB phaseis quasicrystalline (3). For these phases diffraction patterns withup to 18-fold symmetry or higher have been reported (4, 5).Although this structural similarity suggests a possible stabilizingmechanism for the proposed rotated (111) layers, we note that inthe TGB phases the layers are rotated about an in-plane rotationaxis, whereas for the multidomain fcc phase the layer stacks arerotated about a rotation axis normal to the layer plane (Fig. 4B).An in-plane rotation such as in the TGB phase would give rise to

Fig. 1. Synchrotron SAXS (A, B, and C) and SANS (D and E) diffraction patterns of the fcc phase (A) and the quasicrystalline phases Q12 (B,D, and E) andQ18 (C).The SANS patterns have been recorded parallel (D) and normal (E) to the 12-fold rotation axis The circles and lines indicate the position of the reflections thatare compared to the calculated positions for a quasicrystal in Fig. 6. The scattering vector q is given in nm−1; the intensity is displayed on a logarithmic scale.

Fig. 2. Series of synchrotron small-angle X-ray scattering curves for isotropicsamples in a concentration range between 14 and 20%. At concentrations of18 and 20%, the observed peak positions are in good agreement with an fccstructure (space group Fm3̄m). The scattering curves at lower concentrationsare characterized by a suppression of the intensity of the 110 reflection andthe development of a peak at q� ¼ 0.45 nm−1, which for the dodecagonalstructure corresponds to the 20100 reflection.

Fischer et al. PNAS ∣ February 1, 2011 ∣ vol. 108 ∣ no. 5 ∣ 1811

PHYS

ICS

Dow

nloa

ded

by g

uest

on

July

7, 2

020

diffraction patterns that differ considerably from the experimen-tally observed patterns in Fig. 1.

Similar considerations can be made for the structurewith 18-fold diffraction symmetry. Here, a multidomain fcc struc-ture can be proposed that consists of equal numbers of twinned,nonrotated, 20°-rotated, and 40°-rotated (111) layers. To bespecific, we calculated the diffraction pattern of a ðABCÞnðA0B0C0ÞnðA00B00C00ÞnðACBÞnðA0C0B0ÞnðA00C00B00Þn sequence. Alsoin this case, the subscript n denotes the number of layer repeti-tions, the primes indicate 20°-rotated layers, and the doubleprimes indicate 40°-rotated layers. By construction, this diffrac-tion pattern possesses an 18-fold diffraction symmetry. Theschematic structure for n ¼ 1 is shown in Fig. 4 C and F. Thecalculated diffraction pattern for n ¼ 2 is shown in Fig. 6F.

For comparison we have constructed models for quasicrystal-line phases such that their diffraction patterns have 12-foldand 18-fold rotational symmetry with the positions of the reflec-tions being in good agreement with the experimentallyobserved diffraction patterns in Fig. 1. To proceed we note thatthe projection of the (111) layers in the [111] direction can berepresented by a periodic tiling of rhomboedric tiles having a6-fold diffraction symmetry (Fig. 5D). On this tiling one cangenerate nonperiodic tilings with 9-fold (enneagonal) (Fig. 5G)and 12-fold (dodecagonal) symmetry (Fig. 5F). The scalingfactor between the bases of the 6-fold, 9-fold, and 12-fold tilescan be deduced from their hexagonal periodic average structures(PAS) (Fig. 5E) to be 1.485 and 0.536 (6). The full layer structureis then generated by decorating the tiles with micelles. Thetiles and their respective tilings are shown in Fig. 5F for the12-fold, and in Fig. 5G for the 9-fold tiling. Because of the com-

mon PAS, only small rearrangements of the position of themicelles are required for the transition from the FCC to the do-decagonal and enneagonal structure (see Fig. 5 B and C). Fromthe coordinates of the micelles the diffraction patterns arecalculated and are shown in Fig. 6.

We note that the calculated diffraction patterns of the dode-cagonal quasicrystal exhibits reflections, marked in yellow inFig. 6A, that are not present in the diffraction pattern of thefcc multidomain twinned/30°-rotated structure. The appearanceof these reflections in the dodecagonal phase is related to the lossof the Fm3̄mABC stacking and its glide plane upon the transitioninto the Q12 phase. As these reflections are observed experimen-tally, they are a strong indication for the formation of a quasicrys-talline phase. Further, the position of the reflections observedin the perpendicular direction (Fig. 1E) cannot be reproducedby assuming an fcc structure, whereas the calculated diffractionpattern of the dodecagonal quasicrystalline structure shows goodagreement, allowing one to index each of the observed reflec-tions. Also the calculated diffraction pattern of the enneagonal

Fig. 3. Time-resolved microfocus synchrotron SAXS experiment showing the temperature-induced transition from the fcc phase to the Q12 and Q18 phases.The diffraction patterns were recorded in 10-s frames. The dotted line indicates that the involved length scale during the phase transition remains constant.The transition into the Q12 phase proceeds by appearance of an additional set of six reflections after 10 s and subsequently into the Q18 phase by the splittinginto further six reflections after 50 s, as indicated by the arrows.

Fig. 4. Micellar packing in the fcc phase (A and D), in a multidomain0°/30°-rotated, twinned fcc phase (n ¼ 2) with 12-fold symmetry (B and E),and in a multidomain 0°/20°/40°-rotated twinned fcc phase (n ¼ 1) with18-fold symmetry (C and F). (Upper) A view normal to the micellar layers;(Lower) a view perpendicular to the layers.

Fig. 5. Schematic representation of a layer of hexagonally packed polymermicelles (A), an overlay showing the structural relation between an fcc(111) layer and the corresponding layers of the enneagonal and dodecagonalquasicrystals (B and C), a periodic tiling and the tile representing the [111]projection of the fcc phase (D), the tiling and the tiles of the dodecagonalQ12 phase (F) and the enneagonal Q18 phase (G), and an overlay showingthe structural relation between the fcc crystal and the enneagonal anddodecagonal quasicrystals with their respective PAS (E). Different colorsrepresent different layers.

1812 ∣ www.pnas.org/cgi/doi/10.1073/pnas.1008695108 Fischer et al.

Dow

nloa

ded

by g

uest

on

July

7, 2

020

quasicrystal exhibits reflections that are not present in the diffrac-tion pattern of the fcc multidomain twinned/20°-/40°-rotatedstructure. The appearance of these reflections in the experimen-tally measured diffraction patterns of the Q18 phase are a furtherstrong indication for the formation of a quasicrystalline phase. Apeculiarity of the SAXS diffraction patterns is a suppression ofthe innermost reflections of the Q12 and the Q18 phase, whichis related to the opposite X-ray contrast of the micellar core andshell with respect to the solvent. This is different for the neutroncontrast, so that the reflections are visible.

DiscussionThe observation of additional reflections and the agreement be-tween calculated and observed diffraction patterns parallel andperpendicular to the n-fold rotation axis strongly suggest the for-mation of quasicrystalline structures. The diffraction patterns ofsoft lyotropic phases generally do not show many higher-orderreflections due to structural imperfections. For example, thereis a considerable horizontal smearing of the 1000n and 2000n re-flections observed in the experimental diffraction pattern inFig. 1E, which indicates that the micelles on the tile verticesare not exactly located in plane with the other micelles. The largewidth and small number of reflections limit the available struc-tural information. We have in detail considered plausible alter-native structures such as multidomain TGB-type phases thatwould give rise to 12- and 18-fold symmetric diffraction patterns,but in all cases we found that the proposed quasicrystalline struc-tures give the best agreement with the observed diffractionpatterns. We cannot completely rule out the possibility that ayet unknown structure with a very large unit cell, a rather com-plex, hitherto unknownmultidomain fcc (Fm3̄m) structure, or thecoexistence of a yet unknown phase could similarly explain theobserved diffraction patterns. However, we have so far no indica-tions for their existence, and all available experimental data canbe well explained by the formation of the proposed quasicrystal-line structures.

Quasicrystals were first discovered about 25 years ago (7, 8)and are most commonly found in binary and ternary metallicalloys (9), and recently also in binary nanoparticle mixtures(10). They have also been discovered in soft materials such aspolyether dendrons (11) and terblock star copolymers (12, 13).

This report describes quasicrystals that are spontaneously formedby self-assembly in colloidal solutions. As they are water-basedone-component quasicrystals, they are physically and chemicallyvery simple systems. Quasicrystals with 18-fold diffraction sym-metry have previously been unreported for any material.

The existence of colloidal quasicrystals has been theoreticallypredicted for colloids with soft interaction potentials (14). Theywere predicted to be stable at low temperatures in a range ofconcentrations between the disordered state and close-packedcrystals of fcc or hcp type, which is in agreement with our experi-mental observations. The stability was traced to a competitionbetween packing efficiency, favoring the fcc or hcp crystal, andnearest neighbor coordination, favoring quasicrystalline order.Lifshitz and Diamant (15) explained the stability of soft one-com-ponent quasicrystals with the existence of two natural lengthscales together with the presence of three-body interactions.Block copolymer micelles exhibit a soft interaction potential,are inherently characterized by two length scales, i.e., the dimen-sions of the micellar core and the micellar shell (see Fig. 5A), andexhibit interpenetration of polymer chains in adjacent shells mak-ing three-body interactions significant. They thus represent anideal model system to develop a theoretical understanding ofquasicrystalline structure and stability.

The unusual symmetry of quasicrystals has been exploited inrecent years for the fabrication of photonic band gap arrays(16, 17). Owing to their high symmetry, two-dimensional quasi-periodic structures induce and widen the photonic band gap,preventing light within a range of wavelengths from propagatingin any direction. To produce photonic quasicrystals, elaborateelectron beam lithographic techniques are currently used. Ascolloidal quasicrystals are water-based, this opens the way to useestablished colloidal self-assembly wet chemistry routes to gener-ate photonic quasicrystals (18).

Materials and MethodsPolymer Synthesis and Sample Preparation. PI-PEO was synthesized by sequen-tial living anionic polymerization of isoprene and ethylene oxide in THF (19).For the present study, three samples were synthesized and investigated:PI30-PEO125, PI30-PEO120, and PI32-PEO120, where the subscripts denote the de-grees of polymerization. The degrees of polymerization and polydispersitieswere determined by MALDI-TOF-mass spectrometry, size exclusion chroma-

Fig. 6. Diffraction patterns of the dodecagonal phase (A and D), the 0°/30°-rotated multidomain fcc phase (B and E), the enneagonal phase (C), and the0°/20°/40°-rotated multidomain fcc phase (F). A and C are calculated for the h1h2h3h40 reciprocal space layer, D perpendicular to it. The encircled reflectionsare observed experimentally. The reflections encircled in white occur for both the quasicrystalline and the mixed fcc structure. The reflections encircled inyellow occur only for the quasicrystalline structures and are observed experimentally. The reflections for the quasicrystals are indexed based on a set of fivereciprocal base vectors for the Q12 phase and on a set of seven reciprocal base vectors for the Q18 phase.

Fischer et al. PNAS ∣ February 1, 2011 ∣ vol. 108 ∣ no. 5 ∣ 1813

PHYS

ICS

Dow

nloa

ded

by g

uest

on

July

7, 2

020

tography (chloroform), and 1HNMR. The polydispersitiesMw∕Mn were 1;000micelles.

1. Förster S, Plantenberg T (2002) From self-organizing polymers to nanohybrid andbiomaterials. Angew Chem Int Edit 41:688–714.

2. Förster S, et al. (2007) Order causes secondary Bragg-peaks in soft materials.NatMater6:888–893.

3. Chaikin PM, Lubensky TC (1995) Principles of Condensed Matter Physics (CambridgeUniv Press, Cambridge, UK).

4. Navailles L, Barois P, Nguyen HT (1993) X-Ray measurements of the twist grain bound-ary angle in the liquid crystal analog of the Abrikosov phase. Phys Rev Lett 71:545–548.

5. Barois P, et al. (1999) Synchrotron X-ray study of the q-fold quasicrystalline symmetryof the smectic C twist grain boundary phase (TGBc). Eur Phys J B 11:455–462.

6. Steurer W, Haibach T (1999) The periodic average structure of particular quasicrystals.Acta Crystallogr A 55:48–57.

7. Shechtman D, Blech I, Gratias D, Cahn JW (1984) Metallic phase with long-rangeorientational order and no translational symmetry. Phys Rev Lett 53:1951–1953.

8. Levine D, Steinhardt PJ (1984) Quasicrystals: A new class of ordered structures. PhysRev Lett 53:2477–2480.

9. Steurer W, Deloudi S (2008) Fascinating quasicrystals. Acta Crystallogr A 64:1–11.10. Talapin DV, et al. (2009) Quasicrystalline order in self-assembled binary nanoparticle

superlattices. Nature 461:964–967.11. Zeng X, et al. (2004) Supramolecular dendritic liquid quasicrystals. Nature

428:157–160.

12. Takano A, et al. (2005) A mesoscopic Archimedian tiling having a new complexity inpolymeric stars. J Polym Sci Pol Phys 43:2427–2432.

13. Hayashida K, Dotera T, Takano A, Matsushita Y (2007) Polymeric quasicrystal:Mesoscopic quasicrystalline tiling in ABC star polymers. Phys Rev Lett 98:195502.

14. Denton AR, Löwen H (1998) Stability of colloidal quasicrystals. Phys Rev Lett81:469–472.

15. Lifshitz R, Diamant H (2007) Soft quasicrystals—Why are they stable? Philos Mag87:3021–3030.

16. Zoorob ME, Charlton MDB, Parker GJ, Baumberg JJ, Netti MC (2000) Completephotonic bandgaps in 12-fold symmetric quasicrystals. Nature 404:740–743.

17. Steurer W, Sutter-Widmer D (2007) Photonic and phononic quasicrystals. J Phys D40:R229–R247.

18. Ozin GA, Yang SM The race for the photonic chip: Colloidal crystal assembly in siliconwafers. Adv Funct Mater 11:95–104.

19. Förster S, Krämer E (1999) Synthesis of PB-PEO and PI-PEO block copolymers withalkyllithium initiators and the phosphazene base t-BuP4 . Macromolecules32:2783–2785.

20. Lindner P, Zemb Th (2002) Neutrons, X-Rays and Light: Scattering Methods Applied toSoft Condensed Matter (Elsevier, Amsterdam).

21. Roth SV, et al. (2006) Small-angle options of the upgraded ultrasmall-angle x-rayscattering beamline BW4 at HASYLAB. Rev Sci Instrum 77:085106.

1814 ∣ www.pnas.org/cgi/doi/10.1073/pnas.1008695108 Fischer et al.

Dow

nloa

ded

by g

uest

on

July

7, 2

020